Research Inventy: International Journal Of Engineering And ScienceVol.2, Issue 12 (May 2013), Pp 36-50Issn(e): 2278-4721, Issn(p):2319-6483, Www.Researchinventy.Com36Effect of Granite Powder on Strength Properties of ConcreteDr.T. Felix Kala1,Professor and HoD, Department of Civil Engineering, Dr.M.G.R. Educational and Research InstituteUniversity, Maduravoyal, Chennai, Tamil nadu, India – 600095Abstract : This paper focuses on the experimental study of using locally available granite powder as fineaggregate and partial replacement of cement with admixtures in the production of HPC with 28 days strength tothe maximum of 60 MPa. The influence of water cement ratio and curing days on mechanical properties for thenew concrete mixes were premeditated. The percentage of granite powder added by weight was 0, 25, 50, 75 and100% as a replacement of sand used in concrete and cement was replaced with 7.5 % silica fume, 10% fly ash,10% slag and the dosage of superplasticiser added 1% by weight of cement. The test results show clearly thatgranite powder of marginal quantity, as partial sand replacement has beneficial effect on the above properties.The highest strength has been achieved in samples containing 25% granite powder together with admixtures.Based on the results presented in this paper, it can be concluded that concrete mixture can be prepared withgranite powder as an additive together with admixtures to improve the strength of concrete structure.Keywords : concrete properties, fly ash, granite powder, HPC, silica fume, slagI. INTRODUCTIONFine aggregate is an essential component of concrete. The global consumption of natural river sand isvery high due to the extensive use of concrete. In particular, the demand for natural river sand is quite high indeveloped countries owing to infrastructural growth. In this situation some developing countries are facing ashortage in the supply of natural sand. The non-availability of sufficient quantity of ordinary river sand formaking cement concrete is affecting the growth of the construction industry in many parts of the country.Therefore, the construction industries in developing countries are under stress to identify alternative materials toreduce the demand on river sand. In order to reduce the dependence on natural aggregates as the main source ofaggregates in concrete, artificially manufactured aggregates and artificial aggregates generated from industrialwastes provide an alternative for the construction industry . Some alternative materials have already beenused in place of natural river sand. For example, fly ash, slag and lime stone, siliceous stone powder, rock dustand quarry waste were used in concrete mixture as a partial replacement of natural sand . Hence theassumption is granite powder aggregate could be an alternative to natural sand in preparation of concrete.Granite powder, one of the byproducts in granite stone crushing process, not being used for any applicationsother than filling-up low lying areas is identified as a replacement material for river sand in concrete. Thegranite waste generated by the stone crushing industry has accumulated over the years. Only insignificantquantities have been utilized and the rest has been unscrupulously dumped resulting in environmental problems.Presently, all the processing units are disposing this industrial waste by dumping it in open yards, that nearlyoccupying 25% of the total area of the industry.The reduction in waste generation by manufacturing value-added products from the granite stonewaste will boost up the economy of the granite stone industry. The utilization of granite powder in highperformance concrete could turn this waste material into a valuable resource with the added benefit ofpreserving environment. Therefore, this study focused on the possibility of using locally available granitepowder and admixtures in the production of HPC, with 28 days strength to the maximum of 60 MPa. Theadmixtures can be added to cement concrete as a partial replacement of cement along with superplasticiser as awater reducer to get the high performance. Mineral admixtures such as fly ash and slag have the inherent abilityto contribute to the continued strength development and very high durability, the latter through pore refinementand reduced sorptivity. A partial replacement of cement by mineral admixtures, such as fly ash, slag, silicafume, metakaolin, rice husk ash or fillers such as lime stone powders in concrete mixes would help to overcomethese problems and lead to improvement in the durability of concrete . A research  reported that thecompressive strength of concrete incorporating the combination of fly ash and finely ground granulated blastfurnace slag is higher than that of individual concrete. Therefore, based on the above observation, to check thepossibilities of improving the performance of concrete, admixtures were also considered as a partial replacementof cement in this study.
Effect Of Granite Powder On Strength…37However, the selection and dosage of mineral and chemical admixtures are an important considerationfor higher concrete performance. Also, for a better performance of mixture proportions it is required to studyscientifically the properties of proposed concrete. Thus, this research was conducted to evaluate the potential useof granite powder as sand replacement together with admixtures as a partial replacement of cement in theproduction of high performance concrete.II. CONCRETE MATERIALSConcrete is one of the major construction materials being utilized worldwide. Concrete is made usuallyfrom a properly proportioned mixture of cement, water, fine and coarse aggregates and often, chemical andmineral admixtures. Cement is the important binding material in concrete. The most commonly used cement inconstruction today is Portland cement and hence Ordinary Portland Cement of 43 grades has been selected forthe investigation. It is dry, powdery and free of lumps. Aggregates are inert granular materials such as sand,gravel, or crushed stone that are an essential ingredient in concrete. Aggregates, which account for 60 to 75percent of the total volume of concrete, are divided into two distinct categories: fines and coarse. In the presentstudy ordinary blue metal has been used as a coarse aggregate in concrete. Optimum size of the coarse aggregatein most situations was about 19 mm. Sieve analysis of the course aggregates has been done and percentagespassing at different sieves are furnished in Table 1. Fine aggregate is an essential component of concrete. It isdefined as a material that will pass a No. 4 sieve and for the most part be retained on a No. 200 sieve.Table 1 Sieve analysis results of coarse aggregatesThe purpose of the fine aggregate is to fill the voids in the coarse aggregate and to act as a workability agent. Inthe present study, the concrete mixes were prepared using locally available river sand and granite powder. Riversand ranges in size from less than 0.25 mm to 6.3 mm. Fineness modulus and specific gravity of the sand are2.33 and 2.63 respectively. Fineness modulus and specific gravity of the granite powder are 2.43 and 2.58respectively. Sieve analysis was carried out for granite powder and compared with sand, and the results arepresented in Fig. 1.020406080100120Seive Size in mm on Log ScalePercentagePassingSandG Powder0.1 1 10Figure 1 Sieve analysis of fine aggregates for different sieve sizesIt is shown that the amount of fine particles present in granite powder is considerably higher whencompared to the river sand. The constituent materials used for the preparation of the concrete in this study havebeen tested and the details are given in Table 2. Water plays a critical role in the production of concrete,particularly in the amount used. The strength of the concrete increases with less water is used to make concrete.In the present work locally available purified drinking water has been used.Sl.NoSieve Size(mm)PercentagePassing1 25 1002 20 983 16 874 12.5 645 10 266 6.3 037 4.75 00
Effect Of Granite Powder On Strength…38Table 2 Physical properties of constituent materialsSl. No. Materials Description1 Cement Type - OPC 43 GradeSpecific Gravity - 3.15Standard Consistency - 32%Initial Setting Time - 70 MinutesFinal Setting Time - 300 MinutesFineness - 2 %Compressive Strength - 7thday - 41 N/mm2-28thday -62 N/mm22 Blue Metal Specific Gravity - 2.683River Sand Specific Gravity - 2.63Fineness Modulus - 2.334 Granite Powder Specific Gravity - 2.58Fineness Modulus - 2.43On the other hand, admixtures such as silica fume, fly ash, slag and superplasticiser have the inherentability to contribute to continued strength development and very high durability. Silica fume is a byproduct inthe production of silicon metal or ferrosilicon alloys. Because of its chemical and physical properties, it is a veryreactive pozzolan. It has been reported that the mass of silica fume, when used, represents 5 to 15 percent of thetotal mass of the cementitious material, the value of 10 per cent being typical. Moreover silica fume is veryexpensive and wasting a very expensive material is not a good engineering practice . Therefore, in the presentstudy, 7.5% of condensed silica fume was considered as a replacement for cement. The main characteristics ofadmixtures are given in Table 3.Table 3 Chemical compositions and physical properties of silica fume, fly ash and slag (%)Properties Silica Fume Fly Ash SlagSpecific gravity 2.25 2.15 2.95Bulk density, kg/m31000-10000 190-265 1100-11000Specific surface area, m2/kg - 601 607SiO2 95 58.9 33.67Al2O3 0.13 40.1 20.56Fe2O3 4.0 5.2 1.01CaO 0.39 0.89 32.49MgO 0.21 0.27 9.63SO3 - 1.01 0.10Na2O 0.15 0.47 1.22K2O 0.11 0.39 0.48LOl - 1.09 1.19Fly ash is a fine powder recovered from the gases of burning coal during the generation of electricity.Fly ash (Type F) from the Ennoor thermal power plant, Chennai, India was used in the present study. Fly ash isgenerally cheaper than Portland cement and fly ash do not contribute to the slump loss. It has been reported thatthe concrete with 10% fly ash exhibited higher early strength followed by an excellent development of strengthover time . Hence in the present study 10% fly ash was considered as a replacement of cement. Groundgranulated blast furnace slag is often used in concrete in combination with Portland cement as part of blendedcement. Concrete containing ground granulated blast furnace slag develops strength over a longer period,leading to reduced permeability and better durability.
Effect Of Granite Powder On Strength…39Let us now consider the inclusion of ground granulated blast furnace slag in the mix. First of all, slagis generally cheaper than Portland cement. Secondly, it does not contribute to the slump loss. On the other hand,mixes that have more fly ash or more slag develop a lower strength, but this can be compensated by loweringthe ratio of the mass of water to the total mass of cementitious material. It has also been reported that the higherthe amount of slag, the higher the amount of autogenous shrinkage . Hence in the present study, 10% slag isconsidered along with other two admixtures, viz., silica fume and fly ash as a replacement of cement. Groundgranulated blast furnace slag that was supplied by the Andhra Cements, Visakhapatnam, India was used in thisstudy. The use of Superplasticiser in concrete (high range water reducer) has become a common practice. Themain purpose of using superplasticiser is to produce flowing concrete with very high slump in the range of 7-9inches (175-225 mm). The other major application is the production of high-strength concrete at w/cs rangingfrom 0.3 to 0.4 . It increases the compressive strengths of concrete by 50-110% in 3 days, 40-80% in 28 days,and 30-60% in 90 days. Superplasticiser has been added at a rate of 1% of cement mass according to theproducer’s instructions. The properties of superplasticiser as per the manufacturer’s literature are given in theTable 4.Table 4 Properties of superplasticiserSl.No. Properties1234567Specific gravity : 1.220 - 1.225Chloride content : NilRecommended dosage : 2 - 4% of cementApproximate additionalAir Entrainment : 1% at normal dosageSolid content : 40%Compatibility : All types of cement except highalumina cementOperating temperature : 10 - 40%III. EXPERIMENTATIONThis experimental investigation was aimed to introduce high performance concrete by adding thegranite powder together with three admixtures in concrete. Research carried out worldwide has clearlyestablished that suitable addition or replacement of any concrete materials in concrete would lead toimprovement in strength of concrete. In the present study, an experimental investigation was carried out to studythe effect of granite powder together with admixtures in concrete on mechanical properties.The testing of concrete plays an important role in controlling and confirming the quality of cementconcrete works . In this study, total experimentation consisted of compressive strength test, split tensilestrength test, flexural strength test, modulus of elasticity test and water absorption test. Detailed study wascarried out on concrete as per the specifications prescribed in BIS  to ascertain the above properties and thetest procedure adopted are described here independently.3.1 Compressive Strength TestCompressive strength test is the most common test conducted on concrete, because it is easy to performand most of the desirable characteristic properties of concrete are quantitatively related to its compressivestrength. Compressive strength was determined by using Compression Testing Machine (CTM) of 3000 kNcapacity. The compressive strength of concrete was tested using 150 mm 150 mm 150 mm cube specimens.The test was carried out by placing a specimen between the loading surfaces of a CTM and the load was applieduntil the specimen fails. Three test specimens were cast and used to measure the compressive strength for eachtest conditions and average value was considered.3.2 Split Tensile Strength TestKnowledge of tensile strength of concrete is of great importance . Split tensile strength wasdetermined using Universal Testing Machine (UTM) of capacity 600 kN The split tensile strength of concretewas tested using 100 mm 200 mm cylinder specimens. The test was carried out by placing a specimenbetween the loading surfaces of a UTM and the load was applied until the failure of the specimen. Three testspecimens were cast and used to measure the split tensile strength for each test conditions and average valuewas considered.
Effect Of Granite Powder On Strength…403.3 Flexural Strength TestFlexural strength is a measurement that indicates the resistance of a material to deformation whenplaced under a load. The values needed to calculate flexural strength are measured by experimentation, withrectangular samples of the material placed under load in a 3 point testing setup. The strength of a material inbending, expressed as the stress on the outermost fibers of a bent test specimen, at the instant of failure. In aconventional test, flexural strength expressed in MPa is equal to the (equ.1):22PLbd ……… (1)Where, P = the load applied to a sample of test length L, width b, and thickness d.3.4 Modulus of Elasticity TestTo obtain the modulus of elasticity and stress strain behaviour, cylinder specimens of size 100 mmdiameter 300 mm high specimen fixed with compressometer were tested under compression. At every equalload increment, corresponding dial gauge reading in the compressometer was noted and the stresses and strainswere plotted and the modulus of elasticity was calculated for all the concrete mixes. The test specimens werecast and used to measure the modulus of elasticity for each test conditions.3.5 Water Absorption TestThe study of the water absorption, which is closely related to durability of concrete, is veryimportant because deterioration of porous materials like concrete is affected by migration of water. The effect ofa combination of granite powder and admixtures on water penetration of concrete was investigated in theabsorption test. The absorption test was conducted using 500 mm 500 mm 100 mm slabs that were cured at26oC and 38oC water ponding temperatures for 28 days. The slabs were air dried then for 2 days and placed intoa water tank with their bottom 10 mm soaking in water. The water level was monitored in the tank to maintainthe water minimum of 10 mm height. The test involved keeping the slabs into the water for the period of 1 to 2hours and then removed. Measurements were taken using an ordinary inch tape over a cross section of the slabto determine the depth of water rise. This test measures the rate of absorption of water by capillary suction ofunsaturated concrete placed in contact with water. The photographic view of the measurements of waterabsorption in slab specimen is shown in Fig. 2.Figure 2 Measurements of water absorption in slab specimen3.6 Details of Concrete MixThe dosages of different admixtures used in the experimentation were based on the review ofprevious researchers (, , and ). Accordingly, performances of concrete specimens made with 0, 25, 50,75 and 100% granite powder as a replacement of sand with 10% of fly ash, 10% of ground granulated blastfurnace slag, 7.5% of silica fume as a replacement of cement, and 1% of superplasticiser were evaluated. Thelaboratory program conducted in this investigation focused on seven basic mixes and the mixes were designatedwith the grade of concrete and the fine aggregate type used. Mixes incorporating 0% granite powder (100%river sand), 25% granite powder (75% river sand), 50% granite powder (50% river sand), 75% granite powder(25% river sand), 100% granite powder (0% river sand), without any admixtures but only with 100% granitepowder and control concrete (no admixtures and no granite powder) were designated as GP0, GP25, GP50,GP75, GP100, NA100 and CC, respectively. The resultant mixture compositions are shown in the Table 5. ACI
Effect Of Granite Powder On Strength…41mix design method and Bureau of Indian Standards was used to achieve a mix with cube strengths of 60 MPa( and ). Concrete specimens were prepared with w/c ratio of 0.25, 0.30 and 0.35 respectively for M60grade and cured at 35oC (±2oC) water ponding temperature.Table 5 Mix designation with mixture compositionsSl.NoDesignationof MixRiverSand(%)Replacementof sand withgranitepowder (%)Cement(%)Replacementof cementwithadmixtures(%)1. GP0 100 0 72.5 27.52. GP25 75 25 72.5 27.53. GP50 50 50 72.5 27.54. GP75 25 75 72.5 27.55. GP100 0 100 72.5 27.56. NA100 0 100 100 07. CC 100 0 100 03.7 Preparation of Test SpecimensCoarse aggregate was placed in the drum first and batch water was increased to account for theadsorption of the aggregates during rotation. After mixing for 10 to 15 seconds, the fine aggregates with correctproportions was introduced and mixed in for the period of 15 to 20 seconds. This was followed by the final 20%of the water and all the cement were added with fly ash, silica fume and slag, which were mixed in until a totalmixing time of 60 seconds was achieved. The superplasticiser was added 30 seconds after all the other materialsduring the mixing. The various specimens such as cube, cylinder and slab were cast for studying the variation instrength properties due to the replacement of sand with granite powder. Specimens were prepared with water tocementitious materials ratio of 0.25, 0.30 and 0.35 for M60 grade. After 1 day, the specimens were demouldedand cured by water ponding temperature (climate condition) at 35oC (±2oC). The temperature was manuallynoted every hour to find out any variations in 35oC water ponding temperatures. On an average ±2oC variationwas observed in the water ponding temperatures. Different batches were adopted for, 1 day, 7 days, 14 days, 28days 56 days and 90 days of curing ages. The details of different specimens used for the present study are listedin Table 6.Table 6 Details of test specimensMaterial Properties ShapeDimensions of theSpecimens (mm)Compressive Strength(1, 3, 7, 14, 28, 56 and90 days)Cube 150 150 150Flexural Strength(1, 7, 28 and 90 days)Prism 500 150 100Split Tensile Strength(1, 28 and 90 days)Cylinder100 200Modulus of Elasticity(7 and 28 days)100 300Water Absorption(1 and 2 hr)Slab100 500 500
Effect Of Granite Powder On Strength…42IV. TEST RESULTS AND DISCUSSIONAs per the procedure explained above, tests were conducted in various experimental setups to find themechanical properties of new concrete mixture in which granite powder were used in place of river sandpartially as well as admixtures for a partial replacement of cement. The experimental results are presented anddiscussed here for the concrete mixes GP0, GP25, GP50, GP75, GP100, NA100 and CC (comparison purpose)for various operating conditions for M60 grade concrete.4.1 Workability of ConcreteThe workability of concrete for seven mixes was studied and the slump values are furnished in Table 7.The variation in slump values for different concrete mixes was found to be nominal when compared to theconcrete mix with no admixtures (NA100). It is also shown that the slump value increases with the increase inpercentage of granite powder in the concrete mix. However, concrete mixes with granite powder producedhigher slump when compared to the mix with river sand. This improved workability for the mix might be due tothe presence of the more quantity of fine granite powder particles along with admixtures.Table 7 Workability of concrete4.2 Compressive StrengthCompressive strength is considered to be the paramount property of concrete. The effect of introductionof granite powder as a replacement of sand on compressive strength of M60 grade concrete is presented in Figs.3 to 5. The data presented show that the compressive strength of granite powder concretes was higher than thatof reference mix (CC) for all the days of curing. Concrete mixes with admixtures showed increase incompressive strength in all the mixes because of better compatibility than concrete mixes without admixtures. Inthe present study, a significant increase has been observed in the concrete mix with 25% granite powder (GP25)together with admixtures (fly ash 10%, slag 10% silica fume 7.5% and superplasticiser 1%).It can be seen from the Figures that GP25 shows a compressive strength higher than all other concretemixes with granite powder as well as the conventional concrete (CC) for all the days of curing (1 day to 90days). The possible reason for this is that more voids are present in the concrete mixes with higher amount ofgranite powder. More over the crushing strength of granite powder is lower than that of sand and hence theincrease in the content of granite powder has resulted in diminished strength. It is to be noted from the Table 8that the compressive strength of GP25 is 6.12 to 22.14 % greater than that of CC.This shows that the use of admixtures in conjunction with granite powder is a must for harnessing thefull potential benefits of granite powder. The trend of decrease in compressive strength for increase in w/c ratioalso was observed. Previous research indicates that as the water/cement ratio increases, an increase in thestructural porosity of the aggregate–cement paste transition zone occur, which promoted propagation of cracks.Concrete mix Slump in mmGP0 72GP25 75GP50 78GP75 80GP100 80NA100 70CC 70
Effect Of Granite Powder On Strength…43Figure 3 Compressive strength of 0.25 w/c ratio (Variation of concrete mix)Figure 4 Compressive strength of 0.30 w/c ratio (Variation of days of curing)Figure 5 Compressive strength of 0.35 w/c ratio (Variation of days of curing)
Effect Of Granite Powder On Strength…44Table 8 Comparison of compressive strength (MPa) for GP25 and CCW/CMixCompressive Strength (MPa)Testing Age1 Day3Days7Days14days28Days56Days90Days0.25GP25 45.12 57.75 63.50 70.00 74.00 77.00 80.00CC 36.94 49.00 54.00 62.00 67.30 70.50 75.380.30GP25 41.28 52.34 62.00 68.20 71.00 75.60 77.54CC 35.25 46.00 54.00 62.00 62.00 66.85 70.000.35GP25 34.52 42.56 54.25 62.50 66.00 70.50 72.65CC 28.55 36.20 45.10 54.00 58.00 60.00 67.204.3 Split Tensile StrengthThe tensile strength characteristics of concrete are of considerable importance and the split tensiletest is a simple and reliable method of measuring the tensile strength. The variation of split tensile strength withage of curing is shown in Figs. 6 to 8. The specimens of 100 mm diameter cylinder have been tested at the ageof 1, 7, 28 and 90 days. It can be seen from all the Figures that the tensile strength decreased with percentage ofincrease in granite powder in the mix, and the results indicate that the optimum replacement over sand was 25%for all the operating conditions. The reduction in strength may be due to the presence of unfilled micro-voids inthe concrete mixes as the amount of granite powder increased. Conversely, the test results demonstrate the effectof admixtures in all the concrete mixes. It can be seen from Figures that the split tensile strength of granitepowder concretes was increases when admixtures are used, which varies between 2.14 to 6.0 MPa respectivelyfor 1 day, 7 days, 28 days and 90 days of curing.Figure 6 Split tensile strength of 0. 25 w/c ratio (Variation of days of curing)Figure 7 Split tensile strength of 0. 30 w/c ratio (Variation of days of curing)
Effect Of Granite Powder On Strength…45Figure 8 Split tensile strength of 0. 35 w/c ratio (Variation of days of curing)It is to be noted that the split tensile strength of GP25 is 14.88 to 21.95 % higher than that of CC as presented inTable 9. The strength improvement for GP25 shows the effect of admixtures in conjunction with granite powderin concrete mixture. Similar to compressive strength, the trend of decrease in split tensile strength for increase inw/c ratio also was observed for the concrete mixes.Table 9 Comparison of split tensile strength (MPa) for GP25 and CCW/C MixSplit Tensile Strength (MPa)Testing Age1 Day 7 Days 28 Days 90 Days0.25GP25 3.45 4.62 5. 55 5.88CC 2.90 3.80 4.68 5.000.30GP25 2.95 4.35 5.16 5.25CC 2.46 3.56 4.25 4.380.35GP25 2.70 4.00 4.64 4.82CC 2.27 3.28 3.88 4.054.4 Modulus of ElasticityThe investigation on the effect of granite powder replacement on modulus of elasticity isillustrated in Fig. 9 and presented in the Table 10 and 11. The measurements were performed at the age of 7, 28and 90 days, respectively. The data presented in Table 10 show that similar to the strength properties, modulusof elasticity of the concrete mix with 25 % granite powder was found to be higher than that of other percentagesof granite powder concrete mixes as well as reference mix CC for all the days of curing. The range of modulusof elasticity increase in concrete mixes is 4.11 to 6.84 %, 10.16 to 18.54 %, 8.42 to 14.23 %, 6.17 to 8.65 % and0.77 to 3.14 % for GP0, GP25, GP50, GP75 and GP100, respectively as compared with CC for all ages aspresented in Table 10. It is understandable that the increase of modulus of elasticity of concrete mixture with a25 % granite powder (GP25) is 8.85 to 18.89 % higher than that of CC as presented in Table 11. This could beattributed to the cohesiveness of GP25 mix than other concrete mixes.Figure 9 Modulus of elasticity of 0. 35 w/c ratio (Variation of days of curing)
Effect Of Granite Powder On Strength…46Table 10 Modulus of elasticity of concrete mixes at varies curing ageCuring AgeW/CRatioModulus of Elasticity (GPa)Mix DesignationGP0 GP25 GP50 GP75 GP100 NA100 CC7 Days0.2541.42 44.5 43.44 42.66 40.48 38.82 39.3528 days 41.84 44.92 44.0 42.95 40.56 38.78 39.6890 Days 42.62 46.3 45.00 43.82 41.50 40.14 40.747 Days0.3038.12 41.25 40.00 39.10 37.25 35.32 36.5628 days 38.62 41.56 40.20 39.78 37.52 35.72 36.6090 Days 40.45 42.80 42.12 41.25 39.15 38.20 38.857 Days0.3535.16 39.12 37.40 35.22 33.56 32.00 33.0028 days 35.5 39.32 38.52 36.5 34.78 32.45 33.7290 Days 38.42 42.20 40.52 39.00 37.24 35.00 36.14Table 11 Modulus of elasticity development of GP25 compared with CC (%)W/CModulus of ElasticityDevelopment of GP25 (%)Testing Age7 Days 28 Days 90 Days0.25 13.08 13.20 13.640.30 12.82 13.52 10.160.35 18.54 16.60 16.764.5 Flexural StrengthThe effect of granite powder and the performance of admixtures on flexural strength for all concretemixes are presented in Tables 12 and 13, and Figures 10 to 12. From the experimental investigation, it isobserved that the sand replacement by large quantities of granite powder showed lesser flexural strength and for25% sand replacement by granite powder shows increase in flexural strength. It is to be noted that the flexuralstrength of GP25 is 12.5 to 19.88%, respectively, higher than that of reference mix (CC) as presented in Table12 for all the days of curing. It is also shown that the flexural strength increases with the increase in days ofcuring and decreases with the increase in w/c ratios of all concrete mixes.Figure 10 Flexural strength of 0. 25 w/c ratio (Variation of days of curing)
Effect Of Granite Powder On Strength…47Figure 11 Flexural strength of 0. 30 w/c ratio (Variation of days of curing)Figure 12 Flexural strength of 0. 35 w/c ratio (Variation of days of curing)Table 12 Flexural strength development of GP25 compared with CC (%)W/CFlexural Strength Development of GP25 (%)Testing Age1 Day 7 Days 28 Days 90 Days0.25 19.88 16.78 14.80 16.290.30 17.71 16.88 13.27 14.720.35 19.88 19.20 12.50 17.48It can also be seen from the results that the significant improvement in the flexural strength was observed due tothe inclusion of admixtures in the concrete mixes similar to other strength properties. The range of flexuralstrength increases in 3 to 8.73 %, 14 to 21.69 %, 11.43 to 18.34 %, 6.15 to 12.22 % and 0.65 to 4.78 % for GP0,GP25, GP50, GP75 and GP100, respectively, for all ages and different w/c ratios as presented in Tables 13.
Effect Of Granite Powder On Strength…48Table 13 Effect of admixtures on flexural strengthCuring AgeW/CRatioIncrease in Flexural Strength Compared tothe case without Admixtures Mix, CC (%)Mix DesignationGP0 GP25 GP50 GP75 GP1001 Day0.255.64 18.46 16.66 11.28 2.057 Days 6.14 15.57 13.11 12.50 8.1928 days 5.35 16.96 14.64 7.14 2.1490 Days 4.57 14.37 11.43 7.51 6.521 Day0.308.16 21.69 15.49 7.60 4.787 Days 8.73 21.17 18.34 12.22 2.6228 days 6.32 19.54 14.94 9.19 2.2990 Days 6.49 17.32 11.91 8.30 3.611 Day0.355.23 19.69 15.38 6.15 2.767 Days 3.90 17.70 12.64 6.20 3.4428 days 3.00 14.00 14.00 6.40 2.4090 Days 4.02 14.94 12.06 7.66 2.104.6 Water AbsorptionIn general, water absorption in the concrete causes serious problems, which may affect the strength ofthe concrete. In the experimental investigation, the measurements of water rise in the slabs were performed atthe age of 1 and 2 hours. The test results of absorption are presented in Tables 14 and 15. The absorption of theslabs 100 mm 500 mm 500 mm containing granite powder together with admixtures are lower than that ofCC for the tested ages. In the case of concrete mix GP25 the absorption for 1 and 2 hours 14.7 mm and 20.2mm, respectively. It is observed that the reduction in water absorption for GP25 is 8 to 14.2 % compared to theconventional concrete mix CC as presented in Table 14. It could be noted that the variation in absorption fordifferent concrete mixes was found to be nominal for 2 hours of curing when compared to the 1 hour of curing.However, in the case of mix with no admixtures, higher absorption was observed.Table 14 Effect of granite powder on water absorptionHours ofCuringW/CRatioWater Penetration (mm) at 38oC WaterPonding TemperatureMix DesignationGP0 GP25 GP50 GP75 GP100 NA100 CC1 hr0.2513.0 13.0 13.5 14.0 14.5 15.0 14.52 hrs 17.8 17.6 17.8 18.2 19.0 20.0 19.21 hr0.3013.6 13.6 14.2 14.5 15.0 15.0 14.82 hrs 17.9 17.5 19.2 20.4 20.4 20.6 20.41 hr0.3514.2 14.2 14.8 14.6 15.2 15.5 15.02 hrs 19.3 19.0 19.8 20.2 20.8 21.6 21.0
Effect Of Granite Powder On Strength…49Table 15 Comparison of water absorption (mm) for GP25 and CCConcrete MixWater Absorption (mm) forHours of Curingw/c = 0.25 w/c = 0.30 w/c = 0.351hr 2hrs 1hr 2hrs 1hr 2hrsGP25 13.8 18.0 14.5 20.0 14.8 20.6CC 15.0 20.5 15.6 21.5 17.5 22.6GP25 13.0 17.6 13.6 17.5 14.2 19.0CC 14.5 19.2 14.8 20.4 15.0 21.0From the above observations it can be recognized that the new concrete mixture containing 25% granite powderas a replacement of sand together with 27.5% admixtures (7.5% silica fume, 10% fly ash, 10% slag) as areplacement of cement giving maximum performance. Thus GP25 is the best choice among the concretemixtures. Therefore, further study was carried out for GPO, GP25 and compared with control concrete (CC)V. SUMMARY AND CONCLUSIONSAn experimental study on the high performance concrete made with granite powder as fine aggregateand partial replacement of cement with 7.5 % Silica fume, 10% fly ash and 10% slag subjected to water curingis conducted for finding the mechanical properties such as compressive strength, split tensile strength, modulusof elasticity, flexural strength and water absorption characteristics of concrete mixtures. Concrete specimenswere prepared with w/c ratio of 0.25, 0.30, 0.35, for M60 grade concrete mix. The test results show clearly thatgranite powder as a partial sand replacement has beneficial effects of the mechanical properties of highperformance concrete. Of all the six mixtures considered, concrete with 25% of granite powder (GP25) wasfound to be superior to other percentages of granite powder concrete as well as conventional concrete and noadmixtures concrete for all operating conditions. Hence the following conclusions are made based on acomparison of GP25 with the control concrete, CC.The mechanical properties like the compressive strength, split tensile strength, modulus of elasticityand flexural strength particularly for all ages higher than that of the reference mix, CC as mentioned below.There was an increase in strength as the days of curing increased. Compressive strength is 6.12 to 22.14 % greater than that of CC. Split tensile strength is 14.88 to 21.95 % higher than that of CC. Modulus of elasticity is 8.85 to 18.89 % higher than that of CC. Flexural strength is 12.5 to 22.22 % higher than that of CC. The water absorption was about 8 to 14.2 % less than that of conventional concrete mixture.Thus the present experimental investigation indicates that the strength properties of the concrete could enhancethe effect of utilization of granite powder obtained from the crusher units in place of river sand in concrete. Ingeneral, the behavior of granite aggregates with admixtures in concrete possesses the higher properties likeconcrete made by river sand.REFERENCES S. Khalifa Al-Jabri, Makoto Hisada, K. Salem Al-Oraimi and H. Abdullah Al-Saidy, Copper slag as sand replacement for highperformance concrete, Cement &Concrete Composites, 31, 2009, 483-488. Md. Safiuddin, S.N. Raman and M.F.M. Zain, Utilization of quarry waste fine aggregate in concrete mixtures, Journal of AppliedScience Research, 3 (3), 2007, 202-208. Kefeng Tan and Xincheng PU, Strengthening effects of finely ground fly ash, granulated blast furnace slag and theircombination, Cement and Concrete Research, 28 (12), 1998, 1819 -1825. Adam Neville and Pierre-Claude Aitcin, High performance concrete – an overview, Materials and Structures, 31, 1998, 111 –117. M.N. Haque and O. Kayali, Properties of high-strength concrete using a fine fly ash, Cement and Concrete Research, 28, 1998,1445 – 1452. Mladenka Saric-Coric and Pierre-Claude Aitcin, Influence of curing conditions on shrinkage of blended cements containingvarious amounts of slag, ACI Materials Journal, 100, 2003, pp.477-481. V.S. Ramachandran and V. M. Malhotra, Superplasticisers in concrete admixtures handbook (Park Ridge, N.J.: NoyesPublications, 1984) 211 – 268. M.S. Shetty, Concrete Technology-Theory and Practice (S.Chand and Company Ltd, New Delhi, Reprint with corrections, 2007)458 – 503. BIS (Bureau of Indian Standards), Methods of Tests for Strength of Concrete, BIS: 516-1959 (c), New Delhi, India.
Effect Of Granite Powder On Strength…50 A. Camoes, P. Rocha, S. Jalali, De Aguiar, and R. Delgado, High performance concrete using fly ash, Proc. on 3rdInternationalConf. Concrete Technology, Bracil Act SP-207, 2002,15-31. BIS (Bureau of Indian Standards), Plain and reinforcement concrete code of practice, BIS: 456:2000, New Delhi, India.